advertisement

PHYSICAL REVIEW B 79, 134429 共2009兲 Hysteresis and noise in ferromagnetic materials with parallel domain walls Benedetta Cerruti,1 Gianfranco Durin,2,3 and Stefano Zapperi3,4 1Departament d’Estructura i Constituents de la Matèria, Universitat de Barcelona, Martí Franquès 1, Facultat de Física, 08028 Barcelona, Spain 2Istituto Nazionale di Ricerca Metrologica, strada delle Cacce 91, 10135 Torino, Italy 3ISI Foundation, Viale S. Severo 65, 10133 Torino, Italy 4 CNR-INFM, S3, Dipartimento di Fisica, Università di Modena e Reggio Emilia, Via Campi 213/A, I-41100 Modena, Italy 共Received 19 January 2009; published 23 April 2009兲 We investigate dynamic hysteresis and Barkhausen noise in ferromagnetic materials with a huge number of parallel and rigid Bloch domain walls. Considering a disordered ferromagnetic system with strong in-plane uniaxial anisotropy and in-plane magnetization driven by an external magnetic field, we calculate the equations of motion for a set of coupled domain walls, considering the effects of the long-range dipolar interactions and disorder. We derive analytically an expression for the magnetic susceptivity related to the effective demagnetizing factor and show that it has a logarithmic dependence on the number of domains. Next, we simulate the equations of motion and study the effect of the external field frequency and the disorder on the hysteresis and noise properties. The dynamic hysteresis is very well explained by means of the loss separation theory. DOI: 10.1103/PhysRevB.79.134429 PACS number共s兲: 75.60.Ch, 75.60.Ej I. INTRODUCTION The study of ferromagnetic hysteresis represents an open field of current interest due to the applications in magnetic recording technology and spintronic devices.1 From a purely theoretical point of view, the dynamics of disordered magnetic systems represents a central problem in nonequilibrium statistical mechanics. One of the central questions arising in the analysis of ferromagnetic systems is the link between the domain structure and the hysteretic properties such as the coercive field, the power losses, and the noise. From the experimental point of view, it is possible to observe the domain structure on the surface of the sample by magnetooptical techniques, while the bulk behavior is accessible by inductive techniques. Several models have been developed to understand the experimental results, ranging from Ising-type models considering the reversal of a set of interacting spins with2–6 or without disorder7–11 to models focusing on the dynamics of a single domain wall.12–19 These two classes of models represent two extreme situations: spin models are appropriate when dipolar interactions are negligible. On the other hand, in soft magnetic materials magnetostatic effects induce wide parallel domain walls that determine the magnetization properties. The dependence of the hysteresis loop area on the frequency and the amplitude of the applied magnetic field is often referred to as dynamic hysteresis7,20 in the context of thin films and to power losses in bulk materials. In bulk materials, energy dissipation is dominated by eddy currents propagation,1 while in thin films this effect is negligible. This led to the general belief that dynamic hysteresis in thin films is ruled by completely different laws than in bulk samples. The results of the models used to analyze dynamic hysteresis are often interpreted by assuming a universal scaling law for the dependence of hysteresis loop area A on the temperature of the system T, the applied field frequency , and amplitude H0. The experimental estimates of the scaling exponents display a huge variability,21–30 and the validity of a universal 1098-0121/2009/79共13兲/134429共12兲 scaling law is still under debate.31–33 In this respect, it was recently shown that the theory of loss separation developed for bulk materials could be equally well applied to thin films, since the precise nature of the damping 共i.e., eddy currents or spin relaxation兲 does not change the basic equations.34 The Barkhausen effect35 consists in the irregularity of the magnetization variation while magnetizing a sample with a slowly varying external magnetic field. It is due to the jerky motion of the domain walls in a system with structural disorder and impurities.36 Once the origin of the Barkhausen noise 共BN兲 was understood,37 it was soon realized that it could be used as a nondestructive and noninvasive probe to investigate the magnetization dynamics in magnetic materials. From a theoretical point of view, it is a good example of dynamical critical behavior, as evidenced by experimental observations of power-law distributions for the statistics of the avalanche size and duration.3 There is a growing evidence that soft magnetic bulk materials can be grouped into different classes according to the scaling exponents values.38 The Barkhausen noise is also an example of dynamics of a system presenting collective pinning when a quenched disorder is present, and it belongs to the family of the so-called crackling noises.3 This kind of noise is exhibited by a wide variety of physical systems from earthquakes on faults to paper crumpling. So the relative ease to study crackling noise in magnets makes the BN useful to get a deeper insight on different complex systems. The most successful models used to describe the BN have considered the dynamics of a single domain wall,12–19 where the effect of the other domain walls is accounted for by an average demagnetizing field.16 This simplification is justified because the Barkhausen noise is usually measured around the coercive field where the signal is stationary.39 In this regime, the domain walls are reasonably distant from each other and one can assume that their mutual interaction is negligible. The validity of this assumption, however, has never been established firmly. Multiwall effects may in principle affect the domain-walls dynamics and thus dynamic hysteresis and BN. Even if we consider a single domain wall, 134429-1 ©2009 The American Physical Society PHYSICAL REVIEW B 79, 134429 共2009兲 CERRUTI, DURIN, AND ZAPPERI its magnetostatic energy should depend on the number of the domain walls at least in an effective-medium sense. In particular, the demagnetizing factor that plays a crucial role in the BN statistics14 should be correctly evaluated only considering the entire domain structure. An attempt to consider the effect of wall-wall interactions has been made using a spring-block model,40 but this model does not take correctly into account the long-range nature of the dipolar interactions which underlie the multiwall effects. In this paper, we consider a system with many rigid parallel Bloch domain walls and study their motion, driven by an external 共triangular兲 magnetic field, in a disordered material with strong in-plane uniaxial anisotropy. The model is based on the interplay between the dipolar and the external field contributions, in the presence of the structural disorder. Owing to the simplicity of the parallel Bloch configuration, the magnetostatic energy can be treated analytically. We can calculate perturbatively the demagnetizing factor as a function of the structural and geometrical parameters of the system. The perturbative calculation perfectly agrees with the results of the simulations, thus representing a link between a macroscopic measurable quantity and the microscopic dynamics of the system. Moreover, the dynamic hysteresis is investigated by integrating numerically the equations of motion of the domain walls. We analyze the behavior of the coercive field as a function of the applied field frequency and of the disorder density and intensity. Furthermore, with our model we can investigate the Barkhausen noise. We find that the probability distributions for the size, the duration, and the amplitude of the Barkhausen avalanches show a power-law behavior with a cutoff, in qualitative agreement with the available experimental data. These results show that multidomain effects are in principle important, since they give rise to a nontrivial BN and modify the effective parameters 共e.g., the demagnetizing factor兲 describing the motion of a single domain wall. A more complete treatment should involve the dynamics of a system of flexible parallel domain walls, but this goal is beyond the scope of the present work. The manuscript is organized as follows. In Sec. II we present an overview on the energetics of films with parallel Bloch domain walls and we compute magnetostatic, disorder, and external field contributions to the equations of motion of the domain walls. In Sec. III we present the extended perturbative calculation of the magnetic susceptivity and the comparison with the simulation results. Next, we present the results obtained by our simulations for the analysis of the dynamic hysteresis 共Sec. V兲 and of the Barkhausen noise 共Sec. VI兲. Finally, our results are resumed in Sec. VII. II. INTERACTIONS IN A MULTIDOMAIN STRUCTURE Our purpose is to study the motion of n parallel Bloch domain walls in a disordered ferromagnetic system under an external magnetic field driving. The aim is to write an equation of motion for each wall and integrate the system of equations numerically. To this end, we calculate the total forces acting on the domain walls. As we are interested in the macroscopic response, we do not consider the details of the internal structure of the walls and treat only the magneto- z ++++ −−−−++++ −−−−++++ ε d x d y −−−−++++ −−−−++++ −−−− x0 x1 x 2 xn L FIG. 1. 共Color online兲 Sketch of the system parameters, for an array of wall positions 兵x1 , x2 , . . . , xn其. static, the disorder, and the external field contributions. Thus the total force F共k , t兲 acting on the kth wall at time t is given by F共k,t兲 = Fm共k,t兲 + Fdis共k,t兲 + Fext共k,t兲. 共1兲 In Eq. 共1兲, the magnetostatic term Fm共k , t兲 takes into account the interaction between the magnetization and the stray 共magnetostatic兲 field generated by the magnetic charges due to the discontinuity of the magnetization vector at the upper and lower boundaries of the sample, Fdis共k , t兲 models the contribution of structural disorder, impurities, defects and so on, and Fext共k , t兲 describes the interaction between the magnetization and the external magnetic field. A detailed expression for Eq. 共1兲 is obtained by computing the energy E = Em + Edis + Eext for a generic configuration x and then deriving it according to F共k,t兲 = − E . xk 共2兲 In Secs. II A–II C, we will discuss these terms in more detail. A. Magnetostatic force We consider a sample with total length L, height 2d, and thickness ⑀, with n domain walls displaced in the positions 兵x0共t兲 , x1共t兲 , x2共t兲 , . . . , xn共t兲其 at time t, separating n − 1 domains of alternating magnetization. We consider a system with strong uniaxial in-plane anisotropy along the z direction. The even domains have a magnetization equal to M s and the odd ones to −M s, M s being the saturation magnetization of the material 共see Fig. 1 for a definition of the parameters兲. In order to calculate the magnetostatic contribution Fm共k , t兲 to the total force on the kth domain wall at time t, we first compute the magnetostatic energy of the system Em for a generic arrangement of the walls and then derive it with respect to xk. 134429-2 PHYSICAL REVIEW B 79, 134429 共2009兲 HYSTERESIS AND NOISE IN FERROMAGNETIC… -1 The magnetostatic energy Em can be expressed in terms of the demagnetizing field Hd as 冕 共3兲 M · Hddxdydz, ε=0.1 ε=0.01 ε=0.001 -2 1.0×10 2 sample Em/(2µ0MS εLd) 1 Em = − 0 2 1.0×10 where M is the magnetization vector and the integration is taken over the whole sample. Equation 共3兲 can be rewritten as n−1 1 Em = − 0 兺 共− 1兲i 2 i=0 冕 冕 冕 ⑀ xi+1 dx d dy xi 0 dzM s共ẑ · Hd兲, −d -4 1.0×10 0 1×10 since the magnetization lies on the z axis. Using that Hd ជ , where is the scalar potential, it follows that = −ⵜ and therefore n−1 1 Em = 0 兺 共− 1兲i 2 i=0 n−1 冕 冕 冕 冕 冕 ⑀ xi+1 dx xi 0 ⑀ dx xi dzM s −d xi+1 1 = 0M s 兺 共− 1兲i 2 i=0 d dy 共x,y,z兲 z 冕 n−1 dy关共x,y,d兲 − 共x,y,− d兲兴. − g共xi+1,x j兲 − g共xi,x j+1兲兴 − ⑀2关f共xi+1,x j+1兲 0 + f共xi,x j兲 − f共xi+1,x j兲 − f共xi,x j+1兲兴其, n−1 = 兺 共− 1兲 j j=0 ⫻ − 冋冑 冕 x j+1 dx⬘ xj 冕 f共x,y兲 = f共y,x兲 ⑀ = 2冑4d2 + 共x − y兲2 + 共x − y兲 dy ⬘M s 冉 0 ⫻ln 1 共x − x⬘兲2 + 共y − y ⬘兲2 + 共z − d兲2 1 冑共x − x⬘兲2 + 共y − y⬘兲2 + 共z + d兲2 册 g共x,y兲 = g共y,x兲 , n−1 ⫻ 冋 i,j=0 冕 冕 xi+1 x j+1 dx xi xj 冕 冕 ⑀ ⑀ dy 0 冑共x − x⬘兲2 + 共y − y⬘兲2 冑共x − x⬘兲2 + 共y − y⬘兲2 + 4d2 册 . 2 y − x + 冑4d2 + 共x − y兲2 x − y + 冑4d2 + 共x − y兲2 y − x + 冑⑀2 + 共x − y兲2 x − y + 冑⑀2 + 共x − y兲2 冉 − 兩x − y兩 + 共x − y兲 ⑀ ln 3 3 2 冊 冊 , 冑共x − y兲2 + ⑀2 − ⑀ 冑共x − y兲2 + ⑀2 + ⑀ 冊 2 + 关共x − y兲2 + ⑀2兴3/2 . 3 dy ⬘ 0 1 1 − dx⬘ 冉 = 共x − y兲⑀2 ln since the surface charge-density value is M s or −M s on the upper and lower interfaces 共x , y , ⫾ d兲 and 0 elsewhere. The magnetization is uniform inside the domains, thus no volume density of the charge is taken into account. Thus we obtain Em = 0M s2 兺 共− 1兲i+j 共5兲 where r dS 2 1×10 n 1 Em = 0M s2 兺 共− 1兲i+j 兵关g共xi+1,x j+1兲 + g共xi,x j兲 2 i,j=0 The scalar potential is given by the surface integral 共x,y,z兲 = 1 1×10 FIG. 2. 共Color online兲 Normalized magnetostatic energy Em / 共20M s2⑀Ld兲 as a function of the number of domains n, for three different values of the system thickness ⑀ = 0.1; 0.01; 0.001 and for L = 1 and d = 10 calculated for even numbers of domains. Solid lines are guides for the eyes. 共x,y,z兲, z ẑ · Hd = − -3 1.0×10 共4兲 Assuming that ⑀ Ⰶ 2d, as in most of the samples of experimental interest, we can neglect the term 共y − y ⬘兲2 with respect to 4d2 in Eq. 共4兲. Therefore, the result of the integral is given by To give an idea of the behavior of the magnetostatic energy, in Fig. 2 we have plotted Em共t兲 for a sample of fixed length L and d and for three values of the thickness ⑀ = 0.1; 0.01; 0.001, as a function of the number of 共periodic兲 domains. As it can be seen, from a purely magnetostatic point of view, the energy is a decreasing function of the number of domains. In fact, the total number of domains in a sample is determined by the interplay of the magnetostatic term and the domain-wall energy, linearly increasing as a function of n.1 The magnetostatic force on the kth wall at time t is thus 134429-3 PHYSICAL REVIEW B 79, 134429 共2009兲 CERRUTI, DURIN, AND ZAPPERI -3 it can be seen in Fig. 3. For an even number of domains, the central wall experiences a zero force for symmetry reasons. As expected, for a generic 共even or odd兲 number of domains, the effect of the magnetostatic force is to move the walls in the direction that decreases the magnetization, in order to minimize the magnetostatic energy 关see Eq. 共3兲兴. -3 1×10 2 2 Fm(k)/(2µ0MS εL d) 2×10 0 B. Disorder -3 -1×10 -3 -2×10 5 10 15 20 k FIG. 3. 共Color online兲 Normalized magnetostatic force Fm共k , t兲 / 共20M s2⑀L2d兲 on the kth domain wall as a function of k 共dots兲, for a periodic configuration of the domain-walls positions. The sample has n = 21 domains, ⑀ = 0.002, d = 10, and L = 1. The solid line is a guide for the eyes. Fm共k,t兲 = − Em xk共t兲 n−1 = 20M s2 兺 共− 1兲i+k −⑀ 2 冉 i=0 冋 g共xi+1,xk兲 g共xi,xk兲 − xk xk f共xi+1,xk兲 f共xi,xk兲 − xk xk 冊册 U p共x兲 = A exp关− 共x/兲2兴, 共6兲 , where f共x,y兲 y f共x,y兲 =− 冉 = ln x y − x + 冑4d2 + 共x − y兲2 x − y + 冑4d2 + 共x − y兲2 冊 Different sources of inhomogeneities are found in virtually all ferromagnetic materials. The presence of the structural disorder is essential to understand the hysteretic behavior and especially to account for the residual coercive field when the frequency of the external driving field vanishes. Disorder is provided by vacancies, nonmagnetic impurities, dislocations or grain boundaries in crystalline systems, variations in the easy axis between different grains for polycrystalline materials, and internal stresses for amorphous alloys. We consider here only quenched 共frozen兲 disorder that does not evolve on the time scale of the magnetization reversal, which is usually a realistic approximation for ferromagnetic systems. At the beginning of a simulation, we extract the positions of a fixed number n p of pinning centers with a uniform probability distribution all over the sample. Each pinning center interacts with every domain wall by a located potential of the type where x is the distance between the pinning center and the wall, is a correlation length, and the amplitude A is extracted from a uniform distribution, considering that the strength of the pinning centers should vary for structural reasons. In this way, we produce a disordered landscape in which the domain walls evolve. C. External field 共7兲 The interaction between a ferromagnetic system and an external magnetic field H is described by the energy term g共x,y兲 g共x,y兲 =− y x = 2共x − y兲冑⑀ + 共x − y兲 2 Eext = − 0 冑⑀2 + 共x − y兲2 − ⑀ + 2⑀共x − y兲ln 冑⑀2 + 共x − y兲2 + ⑀ y − x + 冑⑀2 + 共x − y兲2 + ⑀2 ln x − y + 冑⑀2 + 共x − y兲2 冉 冕 M · HdV. 共9兲 sample 2 冉 共8兲 冊 冊 In our model, the uniaxial anisotropy and the external time-dependent magnetic field Hext共t兲 are parallel to the easy axis of the sample, and thus parallel or antiparallel to the magnetization. Thus in this case, the total energy is n−1 Eext = 2d⑀0M sHext 兺 共− 1兲i关xi+1共t兲 − xi共t兲兴, − 2共x − y兲2sign共x − y兲. i=0 In Fig. 3, we show the magnetostatic force Fm共k , t兲 calculated at each wall k for a periodic configuration of n = 21 domains. As it could be seen, walls with k of opposite parities are driven in opposite directions, and the absolute value of Fm共k , t兲 is higher for the external walls, which is a finitesize effect tending to reduce the size of the boundary domains. For a large odd number of domains, in the center of the sample, all the Fm共k , t兲 would be equal in magnitude, as and the external field contribution Fext共k , t兲 to the force F共k , t兲 on the kth wall at time t is given by the partial derivative of Eq. 共9兲 with respect to the wall position xk共t兲 and could be thus written as Fext共k,t兲 = 40M sd⑀Hext共t兲共− 1兲k+1 , 共10兲 which depends of course on the parity of the domain wall. 134429-4 PHYSICAL REVIEW B 79, 134429 共2009兲 HYSTERESIS AND NOISE IN FERROMAGNETIC… III. DEMAGNETIZING FACTOR AND MAGNETOSTATIC SUSCEPTIVITY An interesting analytical result that can be obtained from our model is the dependence of the demagnetizing factor on the number n of the parallel domain walls. The parameter enters as a mean-field term in several domain-wall models used to describe the BN.13–16,18 Its precise dependence on the sample geometry is usually approximated considering a uniformly magnetized sample and the domain structure is ignored. Understanding this point is important since determines, for instance, the size dependence of the Barkhausen avalanche distribution.38 The demagnetizing factor can be rigorously defined for uniformly magnetized ellipsoid from the relation Hd = − M. In more general situations, we can define it as an effective quantity linking the average demagnetizing field to the magnetization ⬅ −具Hd典 / M. Here we compute from the magnetic response of the system to a small perturbative external field. Since at equilibrium a small change in the external field is compensated by an increase in the demagnetizing field 共Hd + Hext = 0兲, we can link to the magnetostatic susceptivity = dM / dHext by the relation = 1 / . For an extended system with a large and even number of domains n, the equilibrium configuration consists of a domain-wall array xi = iL n ∀ i, 共note: in what follows, we will omit the t dependence of the functions兲. We can choose a positive perturbative field ␦Hext and thus consider the perturbed walls positions, xi = iL + 共− 1兲i+1u, n x0 = 0, xn = L, that correspond to a 共small兲 increase in the magnetization dM ⬃ nu, with u ⬎ 0, uniformly distributed over the domain walls. Since the calculation of the magnetic susceptivity is quite involved, we discuss it in the Appendix and report here only the final result, = 1 M d , = = Hext ⑀A共n兲 共11兲 where 2.5×10 -4 simulations κ=εA(n)/d 2.0×10 -4 κ 1.5×10 -4 10 n FIG. 4. Demagnetizing factor as a function of the number of domain walls n 共semilogarithmic scale兲: comparison between simulation results and perturbative calculation 共dashed line兲 for d = 400, ⑀ = 0.01, and for unitary L. high and even number of domains and letting the walls relax under an external field that is very low in order to have a displacement from the equilibrium position of the walls of the order of some percents of the distance between nearestneighbor walls. To fulfill the hypothesis under which Eq. 共11兲 is calculated, we use here periodic boundary conditions. As it can be seen, the agreement between theory and simulations is excellent, even if the simulations have been performed for finite samples. The value of the magnetic susceptivity is of the order 1 / = ⯝ 104, which is a realistic value for a ferromagnetic system. It would be very interesting to test the prediction of Eq. 共11兲 with experimental results on materials with low disorder. Finally, it is interesting to notice that the demagnetizing factor = 1 / displays an inverse dependence on the sample length d and a linear dependence on the thickness ⑀. Hence, as expected, reducing the sample aspect ratio leads to an increase in . This fact has been exploited in Ref. 38 to tune and to study its effect on the BN. As final remarks, let us point out that even though no demagnetizing term has been included by hand in the equations of motion, the demagnetization emerges naturally from the interactions between domain walls. Moreover, we will expect the inclusion of the disorder to influence the intrinsic susceptivity but not the demagnetizing field, since the latter only depends on the dipolar fields, at least in the case of 共rigid domain walls兲. A共n兲 = 2关␥ + ln共n兲兴, and ␥ ⯝ 0.577 215. Higher-order corrections in n have been neglected. In Fig. 4 we compare the results of our simulations and the theoretical result of Eq. 共11兲, for a system with d = 400, ⑀ = 0.01, and L = 1—without disorder—by studying as a function of the number of domain walls n 共coinciding with the number of domains in the limit n → ⬁兲. The simulations are performed starting from a periodic configuration of a IV. NUMERICAL MODEL In Secs. II we have calculated the various contributions to the total force acting on each wall 关Eq. 共1兲兴, thus it is now possible to simulate the dynamics of the system. Since the number of the walls is n and we consider in this part closed boundary conditions 共the boundary walls do not move兲, we have to write down n − 2 equations of motion given by 134429-5 PHYSICAL REVIEW B 79, 134429 共2009兲 CERRUTI, DURIN, AND ZAPPERI ⌫ dxk = F共k,t兲 = Fm共k,t兲 + Fext共k,t兲 + Fdis共k,t兲. dt 共12兲 In the following, we set the damping coefficient ⌫ to unity. We integrate these equations using a fourth-order RungeKutta algorithm. The external magnetic field is a saw-tooth signal with rate , being Ḣ ⬀ . We always start our simulations with an M = 0 at Hext = 0 periodical configuration and drive the sample to positive and then to negative saturation. We include the possibility of nucleation and annihilation of the domain walls by fixing a minimum interaction range between two nearest-neighbor walls, namely, ␦min. If two walls get closer than ␦min, we stop them and consider the pair of walls as annihilated. This means that their contribution on the sum involved in the calculation of long-range magnetostatic force 关see Eq. 共6兲兴 and thus their effect on the equations of motion of the other walls is no more considered. Besides, we go on calculating the total force on the annihilated pair of walls. When this force becomes strong enough 共and of the correct sign兲 to let them escape from the range ␦min, we nucleate them and consider again their contribution to the magnetostatic force calculation 关Eq. 共6兲兴. This corresponds to have a nucleation barrier equal to zero. Since we are interested in the study of Barkhausen noise and of the coercive field behavior connected to dynamic hysteresis, this choice does not influence our results, as we have checked. In fact, all the phenomena that we are interested in take place in the central region of the hysteresis loop, namely, the one close to the coercive field Hc, while the choice of the nucleation barrier involves only the region of the cycle close to saturation. Moreover, for the same reason, our results are independent on the choice of ␦min, as long as it is chosen in a reasonable range. V. COERCIVE FIELD AND DYNAMIC HYSTERESIS A. Dynamic hysteresis We first consider the effect of the external field rate on the hysteretic behavior. In Fig. 5共a兲 we show the hysteresis loops obtained for various rates for a system with n = 20 domains 共since from now, we will deal with a reasonably high number of domains, we will use with a slight abuse of terms n for the number of domains兲, where m is the normalized magnetization m = M / M s and h is the normalized magnetic field h = H / M s. As expected from experiments and general considerations, small 共high兲 frequencies correspond to narrow 共large兲 cycles. To quantify this observation, we can focus on the coercive field Hc behavior. In Fig. 5共b兲 we show the dependence of Hc on the field rate . For all the considered values of n in Fig. 5, n = 20, 40, 60 共for a discussion of the behavior of Hc as a function of the number of domains n, see Sec. V B兲, Hc shows an increasing dependence on . The Hc dependence on is quite close to a power law of the form Hc = H p + A1/2 , 共13兲 as suggested for experiments on Permalloy thin films and microstructures fabricated from the same sample31 and by the theory presented in Ref. 12. (a) (b) FIG. 5. 共Color online兲 共a兲 Hysteresis loops for different external field rates, for a system with n = 20 domains and 共b兲 coercive field as a function of the external field rate for three different system sizes n = 20, 40, 60; hc vs dh / dt in a linear plot, in comparison with a square-root fit 共dashed line兲 and the fit with the power loss formula 共continuous line, see text兲. Every point is mediated over 100 realizations corresponding to different disorder configurations. Nevertheless, as it can be seen in Fig. 5共b兲, our curves are best fitted by the loss separation formula,1,34 Hc = H p + Cex关共1 + rḢ兲1/2 − 1兴, r = 4⌫ / 共n20V0兲. 共14兲 where Cex = n0V0 / 2, and Here n0 is the number of active walls in the quasistatic limit 共 → 0兲, V0 is a characteristic field which controls the increase of n0 due to the excess field, is the permeability, and H p is the static 共hysteretic兲 component. The fit parameters values are shown in Table I. The behavior of Hc as a function of suggested in Eq. 共14兲 means that in the adiabatic limit 共low frequencies兲 Hc goes to a nonvanishing value H p that we can interpret as the pinning-dominated quasistatic component due to the structural disorder, while the behavior of Hc in the high rate regime represents the domain-wall dominated dynamic contribution. Moreover, the scaling function of Eq. 共14兲 describes the evolution from the adiabatic to the domain-wall dominated power-law behavior without invoking the mechanism 134429-6 PHYSICAL REVIEW B 79, 134429 共2009兲 HYSTERESIS AND NOISE IN FERROMAGNETIC… TABLE I. Fit parameter values for Fig. 5共b兲. n 20 40 60 Hp Cex r n0 V0 0.024 0.003 6622 183 18 0.0003 0.019 0.003 4752 153 21 0.0003 0.016 0.0036 2989 173 32 0.0002 crossover between domain-wall propagation and nucleation of new domains. In fact, even if the nucleation process is included in our model, besides in a very simplified form, nucleation takes place only in the regions of the hysteresis loops very close to saturation. Thus the cycles are very oblique 关see Fig. 5共a兲兴. Such a kind of hysteresis loops is expected to be dominated by domain-wall motion. (a) B. Role of the number of domains Another interesting issue to analyze is the effect of the number of domains n on the system behavior. We remind here that at the beginning of each simulation, we set the maximum number of domains of the specimen. This number can decrease down to one while driving the system to saturation, and then—increasing the external field—it is completely restored around the coercive field. From a qualitative point of view, keeping constant the other system parameters 共i.e., the physical dimensions of the specimen under study and the pinning centers density and strength f 0兲, a high 共low兲 number of domains corresponds to hysteresis loops with a lower 共higher兲 permeability, in accord with Eq. 共11兲, as it can be seen in Fig. 6共a兲. This happens because the increase in the domain number increases the relative relevance, in the total force balance, of the dipolar contribution. In fact, an absence of collective behavior leads to square-shaped cycles, where the whole magnetization reversal process takes place in a few avalanches. Otherwise, in materials in which dipolar interactions are relevant, oblique hysteresis loops are expected. In our simulations, the coercive field Hc decreases as a function of n, as expected 关see Fig. 6共b兲兴. C. Effect of disorder As we have already mentioned, the presence of the structural disorder has a crucial role in the physics of ferromagnetic systems. Disorder pins the domain walls that thus are not able to move until the external field reaches a sufficient value to overcome the pinning and let the wall move again. Hence we will expect, from this simple argument, that more disordered systems have larger hysteresis loops compared to purer specimens, for the same . We remind here that it is difficult to quantify the disorder contribution in real systems. In our model, we have 2 degrees of freedom to control the disorder: we can tune the density of pinning centers 共by controlling the total number of pinning sites n p兲 and their strength f 0. (b) FIG. 6. 共Color online兲 共a兲 Some hysteresis loops for different system sizes n = 20, 40, 60, for an applied field rate = 1 / 20, and 共b兲 coercive field Hc as a function of the number of domains n. Every point is an average on 100 samples, corresponding to different disorder realization, for an applied field rate = 1 / 1000. The line is a guide for the eyes. In Fig. 7 we show some hysteresis cycles for varying values of the two parameters f 0 关see panel 共a兲兴 and n p 关see panel 共b兲兴. As we can see, their effect on the loops is qualitatively similar, and the behavior for increasing disorder 共i.e., larger cycles for larger disorder兲 is in agreement with the general argument explained above. In Fig. 8, we show the coercive field behavior for increasing disorder intended here as increasing both the values of n p and f 0. As expected, stronger disorder implies higher coercive field. Moreover, it is important to notice that even varying the disorder strength or density, the Hc dependence on the square root of the applied field rate does not change. VI. BARKHAUSEN NOISE The Barkhausen noise is an unavoidable feature of magnetic hysteresis in disordered samples and its statistical properties have been widely studied in experiments and models.38 The experiments in soft ferromagnetic materials have been divided into universality classes depending on the avalanche distributions.38 Experimental results are well described by 134429-7 PHYSICAL REVIEW B 79, 134429 共2009兲 CERRUTI, DURIN, AND ZAPPERI 1 0,5 m 0.022 hc 0 -0,5 -0,2 np=400, f0=.5 f0=2. f0=1.2 f0=.9 -1 -0,1 (a) 0 h 0,1 np=600 f0=.7 0.018 0,2 0 np=400 -0,5 np=600 np=1000 -1 -0,2 2×10 -4 4×10 -4 6×10 -4 8×10 -4 1×10 -3 FIG. 8. 共Color online兲 The reduced coercive field hc dependence on the external field rate dh / dt for a system with n = 40 domains and two different number of pinning centers n p and disorder amplitude f 0. The applied field rate is = 1 / 1000. Data are fitted by Eq. 共14兲. Fit parameters are H p = 0.019, Cex = 0.003, and r = 4752 for n p = 400; H p = 0.017, Cex = 0.0038, and r = 4752 for n p = 600. 0,5 (b) 0 dh/dt 1 m 0.02 -0,1 0 h 0,1 0,2 domain-walls velocity is expected to depend on . We notice that P共v兲 passes from an almost symmetric shape for very high frequencies to an asymmetric one for low frequencies. In the model by Alessandro, Beatrice, Bertotti, and Montorsi 共ABBM兲 model,13 the predicted shape of the amplitude probability distribution is a gamma function P共v兲 ⬀ vc−1e−cv/具v典 . FIG. 7. 共Color online兲 Hysteresis loops for varying: 共a兲 disorder strength f 0共n p = 600兲 and 共b兲 number of pinning centers n p共f 0 = 1.2兲. The rate is = 1 / 50. models involving a single flexible domain wall and ignoring any interactions between different walls. Different universality classes are set by the dominant interactions between parts of the walls. Here we explicitly ignore these local interactions and want to account only for the interactions between walls. In Fig. 9 we show some simulated signals for various rates of the external field. Partial regions are chosen for the signals, corresponding to the same time interval. As it can be seen, our results reproduce a well-known characteristic of the experimental Barkhausen noise. At low frequencies, the signal is composed of separated avalanches, while this property is progressively lost at higher frequencies. In the latter case, the signal appears as a continuous sequence of peaks and the single avalanches are no more distinguishable. We have analyzed the Barkhausen signal considering the distribution of the signal amplitude, avalanche sizes, and durations. The amplitude probability distribution of the magnetic in˙ is a measurable quantity and thus has duction flux rate been often used in order to test the reliability of a model for Barkhausen noise 共see, for instance, Ref. 13兲. In fact, the flux rate is related to the velocity of the domain walls v. In Fig. 10共a兲 we show the rate dependence of the probability amplitude distribution. In the nonadiabatic limit, in fact, the 共15兲 We remind here that this formula is obtained under the assumption that the disorder is a correlated 共Brownian兲 process. The mechanism giving rise to the Barkhausen effect is the domain-walls motion. It can be described as a stationary Markov process then associated with fixed and well-defined values of the magnetization rate imposed to the system and of the permeability of the specimen associated with the part of the hysteresis loop, where the domain-wall motion is assumed to take place. Even if our model is different from the single wall ABBM model, the formula of Eq. 共15兲 is able to fit our probability distributions P共v兲 for high rates, although it does not supply a suitable explanation for the low rate regime 关see Fig. 10共b兲兴. Next, we evaluate the probability distribution for the duration T and the size S ⬅ 兰Tdtv共t兲 of the avalanches. The distributions are shown in Figs. 11共a兲 and 11共b兲. As it can be seen, both distributions display a power-law behavior of the type P共S兲 ⬃ S− and P共T兲 ⬃ T−␣, for almost two decades for the maximum studied size 共n = 60兲, with a cutoff. The scaling exponents are, respectively, ⬃ 1.1 and ␣ ⬃ 1.2. These exponents, however, have never been reported for bulk soft magnetic materials where parallel domain walls are commonly observed.38 This is not surprising as we neglect local interactions and any deformation of the domain wall. It is nevertheless remarkable that just the combined effect of dipolar interactions and disorder yields a power-law avalanche distribution in a multidomain model. The latter 134429-8 PHYSICAL REVIEW B 79, 134429 共2009兲 HYSTERESIS AND NOISE IN FERROMAGNETIC… 1500 ω=1/1300 ω=1/700 ω=1/400 ω=1/300 ω=1/200 ω=1/100 P(v) 1000 500 0 0,001 (a) 0,01 v 80 ω=1/130 c-1 -cv/<v> P(v)=av e FIG. 9. 共Color online兲 Time sequences of Barkhausen noise. The labels indicate the applied field rate. We report portions of simulated signals corresponding to the same time interval. The time is measured considering an integrating time step ⌬t = 0.05. appears, however, essential to recover quantitatively the experimental results in bulk samples.38 It is important to notice that the power-law behavior is believed to be the fingerprint of a system close to criticality. In our case, the physical mechanism involved in keeping the system in that neighborhood is the interplay between demagnetization 共due to dipolar interactions兲 and disorder. However, to completely resolve this issue, it would be necessary to study the dynamics of an array of flexible and interacting domain walls. P(v) 60 40 20 0 (b) 0 0,005 0,01 0,015 v 0,02 0,025 0,03 FIG. 10. 共Color online兲 共a兲 Probability distribution of the signal amplitude 共i.e., of the domain-walls velocity兲 v, for various frequencies of the external magnetic field 共 = 1 / 1300, 1 / 700, 1 / 400, 1 / 300, 1 / 200, 1 / 100, for a system with n = 60 domains. 共b兲 Probability distribution of the signal amplitude for n = 60 and = 1 / 130 fitted with the ABBM function P共v兲 = avc−1 exp共−cv / 具v典兲. VII. CONCLUSIONS The technological and theoretical relevance of the hysteresis in ferromagnetic systems motivates the effort in modeling the phenomenon. Of particular interest is the study of the dynamic hysteresis connected with the power losses of the material and of the Barkhausen noise, which represents a tool for the investigation of the magnetization dynamics. In this paper we have presented a model for the dynamics of a system of parallel and rigid uncharged 共Bloch兲 domain walls, moving in a disordered landscape driven by an external magnetic field. The analyzed configuration of domain walls is a common case both in two- and three-dimensional samples. Our model is based on the interplay between the long-ranged dipolar interactions and the external field and disorder contributions. Due to the simplicity of the wall configuration, we calculated perturbatively the demagnetizing factor and the magnetostatic susceptibility as functions of the geometrical parameters of the system, namely, the thickness, the height, and the number of domains at equilibrium, in the absence of the external magnetic field. The simulation results perfectly agree with the calculations, and we have thus been able to link a measurable macroscopic quantity to the microscopical system behavior. Next, we have investigated the dynamic hysteresis by means of the study of the coercive field behavior obtained by simulating the equations of motion of the walls array. The coercive field displays a power-law behavior as a function of the applied field rate, with an exponent in agreement with experimental available data. Finally, we have analyzed the Barkhausen noise, constructing the probability distributions of the Barkhausen avalanches size and time duration, and found power laws with cutoffs for both the distributions. Moreover, we find that the probability distribution of domain-walls velocity deviates at low driving rates from the ABBM related formula. Since the latter model is based on the motion of a single domain wall, we can conclude that the multidomain effects are important in ferromagnetic systems, since they affect system parameters such as the demagnetizing factor and the behavior of the Barkhausen noise. 134429-9 PHYSICAL REVIEW B 79, 134429 共2009兲 CERRUTI, DURIN, AND ZAPPERI 2 1×10 1 1×10 P(S) For simplicity in the calculations, let us separate the contribution k = j from the others, and rewrite Eq. 共A1兲 as n=20 n=40 n=60 Fm共k兲 = n−1 = 2M s20共− 1兲k+1uk 兺 -1 − ⑀2 -2 1×10 冉 j=1 0,1 (a) + 4M s2 兺 共− 1兲 j+k 1 S j=0 冉 n=20 n=40 n=60 -3 -4 -5 1×10 j 5 4 1×10 1×10 ⫻ FIG. 11. 共Color online兲 共a兲 Probability distribution of the avalanche size S. Dashed line has a slope ⬃ 1.1, and 共b兲 probability distribution of the avalanche duration T, for three different system sizes 共n = 20, 40, 60兲. Dashed line has a slope ␣ ⬃ 1.2 冉 j n−1 Fm共k兲 = 40M s2 兺 j=0 x2 Fm共k兲 = 兺 j=0 冏 ⫻共− 1兲 j+1 冏 uj , 共− 1兲 u j=0 uj = 兺 j=1 冏 冏 u j=0 共A1兲 冊 共A2兲 2 =− 冑4d2 + 共x − y兲2 冉 冑冑 + 2⑀ ln eq 共k兲 is 0 by definition. It folsince the equilibrium term Fm lows: Fm共k兲 xj 2 2g共x j,xk兲 2 f共x j,xk兲 − ⑀ x2k x2k , 2g共x,y兲 = 4关冑⑀2 + 共x − y兲2 − 兩x − y兩兴 x2 eq Fm共k兲 = Fm 共k兲 + ␦Fm共k兲 = ␦Fm共k兲, n−1 冉 where the double derivatives of Eqs. 共7兲 are We can develop the magnetostatic force Fm共k兲 on a generic wall k 关see Eq. 共6兲兴, around its equilibrium position, j+1 冊 ⫻关共− 1兲 juk − 共− 1兲ku j兴, APPENDIX: CALCULATION OF THE MAGNETIC SUSCEPTIVITY Fm共k兲 xj 冊 2g共x j,xk兲 2 f共x j,xk兲 − ⑀2 . 2 xk x2k 2 f共x,y兲 n 2g共x j,xk兲 2 f共x j,xk兲 − ⑀2 2 xk x2k So finally, it results ACKNOWLEDGMENTS B.C. acknowledges the hospitality of ECM Department 共Universitat de Barcelona兲 and a grant from Fondazione A. Della Riccia. 冉 − 40M s共− 1兲k 兺 共− 1兲 ju j -7 1×10 T 冊 2 f共x j,xk兲 2g共x j,xk兲 − ⑀2 uj 2 xk x2k Fm共k兲 = 40M s2uk 兺 共− 1兲 j -6 1×10 (b) 冊册 冊 where we have used the symmetry properties of the derivatives 关see Eq. 共7兲兴. In the last sum, we have included again the kth term since it is null. If we neglect the contribution from the boundaries that could be done since we are in the n → ⬁ case, we can translate j + 1 → j in the first sum, together with the sum index. We obtain 1×10 1×10 共− 1兲 j+1u j u j=0 ⫻共− 1兲 j+1 , 1×10 3 冏 2 2g共x j+1,xk兲 2 g共x j,xk兲 − ⑀ x2k x2k 2 f共x j+1,xk兲 2 f共x j,xk兲 − ⑀2 2 xk x2k n−1 -3 1×10 P(T) 冋冉 0 1×10 1×10 冏 Fm共k兲 Fm共k兲 共− 1兲k+1uk + 兺 xk xj j⫽k ⑀2 + 共x − y兲2 − ⑀ ⑀2 + 共x − y兲2 + ⑀ 冊 . 共A3兲 In order to handle analytically Eq. 共A2兲, let us restrict our study to the limit ⑀ Ⰶ 兩x − y兩 Ⰶ L Ⰶ d, which is the physical case in most ferromagnetic samples. The second derivatives of Eq. 共A3兲 thus become where the last equality descends from the fact that the boundaries of the sample are fixed. 134429-10 1 2 f共x,y兲 =− , x2 d PHYSICAL REVIEW B 79, 134429 共2009兲 HYSTERESIS AND NOISE IN FERROMAGNETIC… 2⑀2 2g共x,y兲 , =− 2 x 兩x − y兩 i and Fm共k兲 could be in this limit rewritten 冉 j the only non-null terms are the ith terms i⬘ with the opposite parity with respect to k that lead to a contribution 冊 2⑀2 ⑀2 共− 1兲 j+k + 兩x j − xk兩 d Fm共k兲 = 40M s2 兺 − ⫻关共− 1兲kuk − 共− 1兲 ju j兴. n Fm共k兲 = − =− 兺i 80M s2⑀2uk 冉 i n/4 = − 4␣共− 1兲k 兺 i=1 − L Fm共k兲 = where 冊 1 2 + 共− 1兲i+k 兩xi − xk兩 d 兺i 80M s2⑀2un 共− 1兲kA共n兲, L 冋 冉冊 A共n兲 = 2 ␥ + ln 共A6兲 册 n + 2 ln共2兲 , 4 by using the sum of a harmonic finite series of odd terms, where ␥ = 0.577 215. So finally 册 n + 2 ln共2兲 = 2关␥ + ln共n兲兴. 4 The energy term due to the external magnetic field is given by Eq. 共9兲, and in this case could be written as Eext = − 40M sHextd⑀ 兺 ui . i Therefore, Fext共k兲 is given by Fext共k兲 = − 兺i 关共− 1兲i − 共− 1兲k兴 80M s2⑀2un 1 2i − 1 冋 冉冊 So only the walls with the opposite parity with respect to k will contribute to Fm共k兲. Thus the even 共odd兲 walls that have a negative 共positive兲 displacement will experience a positive 共negative兲 force, recalling the wall to the equilibrium position. So, starting from Eq. 共A6兲, we can write d 1 i = − 2␣共− 1兲k ␥ + ln ⫻关共− 1兲 − 共− 1兲i兴. Fm共k兲 = n/2 Fm共k兲 = − 4␣共− 1兲k 兺 共− 1兲i 兩xi − xk兩 k 40M s2⑀2u Since n → ⬁, we could consider k in the middle of the sample and write i⬘=1 that means that every wall i contributes with a term of sign 共−1兲i+1. Since the most important contribution in the sum of Eq. 共A5兲 is due to the nearest neighbors, if k is odd 共even兲 and has thus a positive 共negative兲 perturbation on the position, it will be subject to a negative 共positive兲 magnetostatic force, recalling the wall to the equilibrium position. Considering the case with all the perturbations ui = u, ∀i, the magnetostatic force becomes Fm共k兲 = 40M s2⑀2u 兺 − i⬘=0 共A5兲 共− 1兲i+k 共− 1兲kuk 兩xi − xk兩 兺i 1 . 兩i − k兩 Fm共k兲 = ␣共− 1兲 共− 2兲 兺 k To have some insight on Eq. 共A5兲, we can study the effect of the magnetostatic force in two simplified situations Let us imagine that all the walls are fixed but the kth. Thus Eq. 共A5兲 can be rewritten as 80M s2⑀2 1 关共− 1兲i+k − 1兴, 兩i − k兩 Fm共k兲 = ␣共− 1兲k 兺 共A4兲 Eext xk 40M sHextd⑀ 兺 ui 1 关共− 1兲i − 共− 1兲k兴, 兩i − k兩 i = 共− 1兲k+1uk = 共− 1兲k+140M sHextd⑀ . using the definition xi = iL / n. Since L Ⰶ d and n / 兩i − k兩 ⱖ 1 ∀ i, k, we can approximate 80M s2⑀2un 1 Fm共k兲 ⯝ − 兺i 兩i − k兩 关共− 1兲i − 共− 1兲k兴 L = ␣兺 i Since at the equilibrium the total force F = 0, in the absence of disorder it must be Fm共k兲 + Fext共k兲 = 0 1 关共− 1兲i − 共− 1兲k兴, 兩i − k兩 = 80M s2⑀2un 共− 1兲kA共n兲 L + 共− 1兲k+140M sHextd⑀ , defining ␣ = 80M s2⑀2un / L. In the sum 134429-11 PHYSICAL REVIEW B 79, 134429 共2009兲 CERRUTI, DURIN, AND ZAPPERI from which follows: Hext = M= So finally, we can calculate the magnetic susceptivity , 2⑀uA共n兲M sn . Ld = The magnetization M could be written as M M d , = = Hext Hext ⑀A共n兲 共A7兲 which was our goal. G. Bertotti, Hysteresis in Magnetism 共Academic Press, San Diego, 1998兲. 2 J. P. Sethna, K. Dahmen, S. Kartha, J. A. Krumhansl, B. W. Roberts, and J. D. Shore, Phys. Rev. Lett. 70, 3347 共1993兲. 3 J. P. Sethna, K. A. Dahmen, and C. R. Myers, Nature 共London兲 410, 242 共2001兲. 4 E. Vives and A. Planes, Phys. Rev. B 50, 3839 共1994兲. 5 E. Vives and A. Planes, J. Magn. Magn. Mater. 221, 164 共2000兲. 6 E. Vives and A. Planes, Phys. Rev. B 63, 134431 共2001兲. 7 B. K. Chakrabarti and M. Acharyya, Rev. Mod. Phys. 71, 847 共1999兲. 8 M. Acharyya and B. K. Chakrabarti, Phys. Rev. B 52, 6550 共1995兲. 9 S. W. Sides, P. A. Rikvold, and M. A. Novotny, Phys. Rev. E 59, 2710 共1999兲. 10 H. L. Richards, M. A. Novotny, and P. A. Rikvold, Phys. Rev. B 54, 4113 共1996兲. 11 S. W. Sides, P. A. Rikvold, and M. A. Novotny, Phys. Rev. E 57, 6512 共1998兲. 12 I. F. Lyuksyutov, T. Nattermann, and V. Pokrovsky, Phys. Rev. B 59, 4260 共1999兲. 13 B. Alessandro, C. Beatrice, G. Bertotti, and A. Montorsi, J. Appl. Phys. 68, 2901 共1990兲. 14 S. Zapperi, P. Cizeau, G. Durin, and H. E. Stanley, Phys. Rev. B 58, 6353 共1998兲. 15 P. Cizeau, S. Zapperi, G. Durin, and H. E. Stanley, Phys. Rev. Lett. 79, 4669 共1997兲. 16 J. S. Urbach, R. C. Madison, and J. T. Markert, Phys. Rev. Lett. 75, 276 共1995兲. 17 O. Narayan, Phys. Rev. Lett. 77, 3855 共1996兲. 18 M. Bahiana, B. Koiller, S. L. A. de Queiroz, J. C. Denardin, and R. L. Sommer, Phys. Rev. E 59, 3884 共1999兲. 19 S. L. A. de Queiroz and M. Bahiana, Phys. Rev. E 64, 066127 共2001兲. 20 T. A. Moore and J. A. C. Bland, J. Phys.: Condens. Matter 16, 1 4ud⑀ M sn 2uM sn . = 2dL⑀ L R1369 共2004兲. Raquet, R. Mamy, and J. C. Ousset, Phys. Rev. B 54, 4128 共1996兲. 22 Y.-L. He and G.-C. Wang, Phys. Rev. Lett. 70, 2336 共1993兲. 23 C. N. Luse and A. Zangwill, Phys. Rev. E 50, 224 共1994兲. 24 Q. Jiang, H.-N. Yang, and G.-C. Wang, Phys. Rev. B 52, 14911 共1995兲. 25 J.-S. Suen and J. L. Erskine, Phys. Rev. Lett. 78, 3567 共1997兲. 26 W. Y. Lee, B.-Ch. Choi, Y. B. Xu, and J. A. C. Bland, Phys. Rev. B 60, 10216 共1999兲. 27 B. C. Choi, W. Y. Lee, A. Samad, and J. A. C. Bland, Phys. Rev. B 60, 11906 共1999兲. 28 W. Y. Lee, Y. B. Xu, S. M. Gardiner, and J. A. C. Bland, J. Appl. Phys. 87, 5926 共2000兲. 29 W. Y. Lee, A. Samad, T. A. Moore, J. A. C. Bland, and B. C. Choi, Phys. Rev. B 61, 6811 共2000兲. 30 J.-S. Suen, M. H. Lee, G. Teeter, and J. L. Erskine, Phys. Rev. B 59, 4249 共1999兲. 31 C. Nistor, E. Faraggi, and J. L. Erskine, Phys. Rev. B 72, 014404 共2005兲. 32 L. Santi, R. Sommer, A. Magni, G. Durin, F. Colaiori, and S. Zapperi, IEEE Trans. Magn. 39, 2666 共2003兲. 33 B. Cerruti and S. Zapperi, Phys. Rev. B 75, 064416 共2007兲. 34 F. Colaiori, G. Durin, and S. Zapperi, Phys. Rev. Lett. 97, 257203 共2006兲. 35 H. Barkhausen, Phys. Z. 20, 401 共1919兲. 36 G. Durin and S. Zapperi, The Science of Hysteresis: Physical Modeling, Micromagnetics, and Magnetization Dynamics 共Academic, Amsterdam兲, Vol. 2, Chap. 3, pp. 181–267 共2006兲. 37 H. J. Williams and W. Shockley, Phys. Rev. 75, 178 共1949兲. 38 G. Durin and S. Zapperi, Phys. Rev. Lett. 84, 4705 共2000兲. 39 G. Durin and S. Zapperi, J. Stat. Mech.: Theory Exp. 共2006兲 P01002. 40 K. Kovács, Y. Brechet, and Z. Néda, Modell. Simul. Mater. Sci. Eng. 13, 1341 共2005兲. 21 B. 134429-12